Concrete international / January 2011 41
by Dale P. bentz, Casimir J. bognaCki, kyle a. riDing, anD ViCtor H. Villarreal
Hotter Cements, Cooler Concretes
Finer cements may require engineered solutions to reduce the maximum temperature rise in concretes
Many things have changed in the concrete industry during the past 50 years, including the basic characteristics of portland cementthe main component of concretes binder phase. In general, phase composi-tion, fineness, and alkali levels have each changed in a manner that results in higher early strengths and higher early-age heat generation (so-called hotter cements). The objective of this article is to examine trends in cement production, and provide practical solutions to producing cooler concretes with hotter cements.
Trends in cement production have mainly been driven by the desire for generating high early strengths to support fast-track construction. To a large extent, this has been achieved by finer grinding of the cement to enhance early-age hydration and strength development. Figure 1 presents two sets of survey data concerning cement finenessthe first showing mean fineness values from three surveys as presented by the Portland Cement Association1 and the second based on individual results from the Cement and Concrete Reference Laboratory (CCRL) (www.ccrl.us) proficiency sample program compiled during the past 40 years.
While one can argue that there is no guarantee that the cements selected by CCRL are representative of the cements available from the industry as a whole, taken together, all of the results in Fig. 1 clearly indicate the trend of increasing cement fineness. Both regression lines in Fig. 1 have a statistically significant non-zero slope that indicates an increase in fineness of about 10 m2/kg every 10 years. It may have been unlikely that this trend could continue, as the AASHTO M85-04 specification contained a maximum fineness limit of 420 m2/kg for Types I, II, IV, and V cements. However, when the ASTM International and AASHTO standards were recently harmonized in 2009, the only maximum fineness limit that was established was a value of 430 m2/kg for Type II(MH) and Type IV cements, with no maximum limits being established for Type I, II, or V cements.2
While increased fineness produces increased early-age strengths, it also produces a greater heat release at early agesboth due to increased rates of hydration. To demonstrate this nearly one-to-one relationship, Fig. 2 presents mortar cube compressive strength and isothermal calorimetry results, both for ordinary portland cement mortar mixtures prepared with six different fineness cementsall based on the same clinkerwith finenesses ranging from 613 to 302 m2/kg.3 The mortar cubes for compressive strength were demolded after 1 day and stored in saturated limewater at 73.4F (23C) until testing. For the three ages examined in the study, as fineness increases proceeding from left to right in the graph, there is nearly a linear relationship between heat release and strength. At each of these three ages, finer cements are stronger, but they are also hotter.
While it seems clear that cements are getting hotter, the natural follow-up question is whether this is cause for concern. If a wide range of cement finenesses were available, the answer would be perhaps not. Because most cement producers are hesitant to produce a wide range of products, however, the same Type I/II cements that
Fig. 1: Changes in Blaine fineness of cements from the 1950s to the present day. Individual regression lines are provided for the Type I survey and CCRL Type I or I/II data sets only
42 January 2011 / Concrete international
are manufactured for high early-age strength applications, such as high-rise construction, are also being employed in pavements and bridge decks, where long-term durability is often more critical than early-age strength. ASTM C150 specifically includes a low heat of hydration cement designated as Type IV ( 250 J/g cement for 7 days heat of hydration); to the authors knowledge, there are currently no Type IV cements being produced in the U.S. In addition, for Type II cements, there is a low heat of hydration option that can be specified ( 290 J/g cement for 7-day heat of hydration); this approach is now employed in practice by state transportation agencies and other specifiers.
In fairness, it should be noted that some coarser cements are locally available, such as the 302 m2/kg cement (Fig. 2) currently produced in California. When available, such a coarser cement can be effectively blended with a finer cement to produce a range of cement finenesses and achieve a wide range of strength and heat release values as indicated in Fig. 2.3 In many parts of the
U.S., its difficult to find a cement with a fineness of less than 360 m2/kg. Given that coarser cements are not readily available, the next question is whether the use of finer cements produces adverse effects in concrete. When high temperatures are produced in a curing concrete element, three issues of major concern are thermal cracking, reduced ultimate (in-place) strengths, and delayed ettringite formation (DEF).4
A ReAl-WoRld exAmpleIn fall 2006, the Port Authority of New York & New
Jersey (PANYNJ) was assigned the task of building the Freedom Towernow called Tower Oneat the World Trade Center site in New York City. The tower foundations, which required 12,000 and 8500 psi (83 and 59 MPa) concretes, were under construction at the time. The cementitious material contents for the 12,000 and 8500 psi (83 and 59 MPa) mixtures were respectively 1250 and 1040 lb/yd3 (742 and 617 kg/m3), and the portland cement contents were respectively 700 and 520 lb/yd3 (415 and 309 kg/m3). The foundations exhibited significant cracking within the first 48 hours. The internal temperature of an 8500 psi (59 MPa) foundation placement made in November 2006 was monitored and found to have reached about 170F (77C) at 24 hours, remaining above 160F (71C) for more than a week (Fig. 3). PANYNJ was alarmed that such a high temperature had been reached in November. What would the internal cure temperatures be in the summer months?
The tower core and structural walls for the tower are up to 6 ft (1.8 m) thick. For these, the concrete temperature rise was restricted to 160F (71C) to minimize strength reduction and the potential for DEF; the temperature difference between the core and surface temperatures was restricted to 35F (19C). The tower core required a 14,000 psi (97 MPa) mixture. Before the mixture was approved, 6 x 8 x 10 ft (1.8 x 2.4 x 3 m) blocks had to be placed and the temperature rise recorded, with companion test cylinders being made for determining strength and modulus of elasticity. The evaluated concrete mixture proportions and mechanical properties measured at 56 days are given in Table 1.
The core temperature profiles for the mixtures are given in Fig. 4. Mixture 1 had a cement content of 695 lb/yd3 (412 kg/m3) and reached a peak temperature of 182F (83C) in 24 hours. Mixture 2 had 264 lb/yd3 (157 kg/m3) of cement and reached a peak temperature of 162F (72C) in 40 hours. Based on these results, Mixture 2 was selected.
After about 6 months, 4 in. (102 mm) diameter cores were taken from the center of the blocks and 1 ft (0.3 m) from an outside face by vertically drilling from the top. Horizontal cores were also taken. All of the core results
Fig. 2: Mortar cube compressive strength versus heat release at three different ages for mortars prepared with different fineness cements.3 For each data series, fineness increases from left to right, with measured average particle sizes of 17.8 m, 12.5m, 11.2 m, 9.1 m, 7.9 m, and 6.8 m (1 m = 3.9 105 in.)
Fig. 3: Mass concrete core temperature
Concrete international / January 2011 43
for a given mixture were very consistent, as indicated by their respective strength ranges. For Mixture 1, the compressive strengths ranged from 12,320 to 12,880 psi (85 to 89 MPa) with an average of 12,640 psi (87 MPa). This was 30% lower than the 56-day results for corre-sponding cylinders cast on the day of the placement and cured in accordance with ASTM C31. The cores from Mixture 2 averaged 15,780 psi (109 MPa) with a range of 15,470 to 16,380 psi (107 to 113 MPa). This was 9% lower than the 56-day cylinders cast on the day of the placement.
The strength differences between cores and cast cylinders were attributable to three potential primary factors: consolidation, damage to cores during drilling, and the curing temperature during the initial 24 hours. Consolidation should not have been a significant factor because the concrete blocks contained no reinforcement and the mixture was placed at about an 11 in. (280 mm) slump. To assess how much reduction in strength was potentially due to coring for a nominally 14,000 psi (97 MPa) concrete mixture, PANYNJ cast 10 in. (254 mm) slabs in the laboratory with companion cylinders being cast; both cylinders and slabs were cured in the laboratory in accordance with ASTM C31. Four inch (102 mm) diameter cores were taken from the slabs at 7 and 56 days. The cores taken at 7 days were also cured in accordance with ASTM C31. The 56-day compressive strengths produced by the cores and companion cylinders were virtually the same. Therefore, the lower core strengths taken
from the original mock-up were not due to coring issues and were most likely due to the higher temperatures in the blocks (as the concrete was not cured in accordance with ASTM C31).
The adverse effects of high curing temperatures during the initial week should be considered when specifying high-strength and/or mass concrete. This is in agreement with the Portland Cement Associations Design and Control of Concrete Mixtures,